Polyaniline synthesis was confirmed from Fourie transformed infrared spectrometry test which the result is depicted in figure . As we can see in the Fig. the observed picks in 1565 cm and 1485 cm and 1248 cm peaks are ⅟ ⅟ ⅟ related to bending and extension vibratory of C-H bond. Also, the observed peak at 1109 cm is ⅟ related to extension vibratory of carbon nitrogen joint which shows the correct preparing process of polyaniline in conductive form. Cloth surface coverage with polyaniline further studied by scanning electron microscopy that is shown in the figures 2 and 3 for untreated and pretreated cloths respectively. In the Fig. left, the dense clothe before polymerisation process and in right portion of Fig. , the dense cloth after the polymerization process are depicted. On the other hand, in the Fig. left, the base treated polyester cloth before the polymerisation process and in Fig. right, pretreated polyester cloth after the polyaniline coating are shown. As we can see from the comparison the pre-treated cloth showed much more uniformity and homogeneity of the polyaniline coverage.